Effect of Age Cement Type Temp on Silica Fume Concrete
Embed Size (px)
Transcript of Effect of Age Cement Type Temp on Silica Fume Concrete
EFFECT OF AGE, CEMENT TYPE, MODERATE SHIFT IN TEMPERATURE ANDWATER-CEMENT RATIO ON SELF-DESICCATION IN SILICA FUMECONCRETE
Bertil Persson, M.Sc., Lic. Tech., CIV.ENG.Div. Building Materials, Lund University, Box 118, 221 00 Lund
This article outlines an experimental and numerical study on theeffect of cement type, silica fume, w/c, age and moderate shift oftemperature on self-desiccation and strength of concrete. For thispurpose 81 sealed cylinders made of 9 concretes with w/c varyingbetween 0.32 and 0.50, based on two types of Portland Cement,were manufactured. Five per cent silica fume was used in one thirdof the concretes as calculated on the basis of the cement content.Self-desiccation was studied after sealed curing at three differenttemperatures. The measurement was done at 1 and 6 months ageat three temperatures. The results indicated high influence of age,cement type and w/c on self-desiccation. The study was performedat Lund Institute of Technology, Lund University 1997-1998.
Keywords: Alkali-effect, Compressive strength, High PerformanceConcrete, Internal Relative Humidity, Self-desiccation, Silica fume.
The chemical shrinkage that takes place during hydration of water to cement is the fundamentalcause of self-desiccation /1/. The specific volume of the hydrated water in the gel of concrete isreduced by about 26% compared with the specific volume of water in the capillary pores /2/.Especially at low w/c < 0.38 the effect of self-desiccation becomes more pronounced due tothe decreased size of the capillary pores /3/. Self-desiccation influences the properties of theyoung concrete as well as the long-term behaviour of the concrete, i.e. deformations, stabilityand durability. Due to the self-desiccation concrete with low w/c deforms even with sealedcuring, free of imposed stresses (autogenous shrinkage) /4,5/. Furthermore low-w/c concreteespecially with silica fume may exhibit a rather low long-term increase of the compressivestrength due to self-desiccation, which may influence the long-term stability and durability /6/.Favourable parameters related to self-desiccation are low internal relative humidity close to thereinforcement bars, which may decrease the rate of corrosion /7/. Frost resistance and scalingof materials and structures is clearly improved due to self-desiccation since an air-filled volumeis created due to the chemical shrinkage as mentioned above /8-10/. A low amount of built-in
2moisture during the construction time is another favourable property of low-w/c concretescaused by self-desiccation /11-13/.
1.2 Objective of the study
The main aim of the study was to ascertain the influence of cement type, w/c, silica fume, ageand moderate shift in temperature on internal relative humidity, RH, due to self-desiccation inconcretes with w/c varying between 0.32 and 0.50. The effect of self-desiccation on the RHproperties was secured by studying concrete at 1 and 6 months age. The effect of cement typewas ascertained by studies on low- and normal-alkali cement. Half of the number of specimensthat were made with normal-alkali cement was blended with 5% silica fume as calculated onthe basis of the cement content. Finally, the effect of temperature changes was studied at threelevels varying between 18.5 C and 23 C. Another aim was to observe the effect of cementtype, silica fume and temperature on the compressive strength of concrete with sealed curing.
1.3 General layout of the work
Nine different types of concrete were examined. After sealed curing at three differenttemperatures (18.5, 20.5 and 23 C) the concrete strength was tested at 1 months age. RHwas measured on pieces of crushed concrete at the mentioned temperatures at 1 and 6 monthsage. The density of the concrete was studied in the fresh state and after sealed curing for 28days.
2.1 Materials and studied concretes
The concretes had good rheological properties. The 28-day 100-mm cylinder compressivestrength exceeded 20-40 MPa (comparable with 25-50 MPa 150-mm cube strength). The mixdesign was based on theoretical optimisation of the grading curve in the fresh concrete in orderto obtain good workability /14/. The w/c varied between 0.32 and 0.50. The slump of theconcretes varied between 80 and 180 mm. It was possible to mix, transport and cast HPC withexisting methods. Low-alkali and normal-alkali cement was used. Appendix 1 gives thechemical composition of the cements /15/. Nine types of concrete were studied, 9 cylinders ofeach quality, in all 81 cylinders. Properties of the aggregate are given in Appendix 2 /16/. Firstof all the dry material was mixed for minute. Then the water with air-entrainment was addedand mixed for another minute. Finally, the plasticisers were added and mixed for 3 minutes.Workability, density and air-content of the concretes were studied in the fresh state. Appendix3 shows the mix design of the concretes and the main properties in the fresh and the curedstate.
2.2. Specimens and curing conditions
Density, compressive strength and self-desiccation after sealed curing of the concretes werestudied for cylinders 200 mm long and 100 mm in diameter. The mixing of the material took
3place at 22 C. Directly after mixing, one third of the moulds with concrete were stored atconstant temperatures (18.5 C) in a climate chamber, one third at 20.5 C and one third at 23C. After demoulding at one days age the specimens were immediately sealed from moistureby insulation with 3 mm plastic tubes and replaced in the climate chambers where the initialcuring took place. The weight of the cylinders was established before and after the 28-daytests.
2.3 Experimental methods
The cylinder with the plastic tube was weighed. Then, all concrete cylinders were weighed andmeasured separately. The plastic tube was weighed separately in order to detect any increasedue to moisture uptake. The cylinder was placed centric in a hydraulic press device and theloading applied at 1 MPa/s. Minimum 5-mm fragments from the concrete used in thecompressive testing were filled in glass tubes 150 mm long and 22 mm in diameter. Thetemperature of the fragments and that of the climate chamber were adjusted to each other for 1day. Then the internal relative humidity, RH, was measured by a dew-point meter (Protimeter)for 22 h. The probe of the dew-point meter was entered into the glass tube and tightenedagainst the glass with an expanding rubber ring.
3. INTERNAL RELATIVE HUMIDITY, RH, AT 1 MONTHS AGE
3.1 Density and compressive strength
Appendix 3 provides the density and compressive strength after curing for 28 days. The fall inair-content was estimated from the difference in density between the fresh and the cured stateof the concrete. The losses of air content in the concrete were quite large, Appendix 3.However, the high amount of air-entrainment was required in order to maintain goodworkability at the low w/c (low mixing water content) shown in Appendix 3. Otherwise muchlarger cement content would have been required. The air-entrainment replaced a good part ofthe water during the casting. The compressive strength decreased slightly with a moderateincrease of the curing temperature, especially at w/c= 0.38, i.e. between 0.5 and 2.5 MPa/C.Figure 1 shows the air content in the concretes in the fresh state and after curing and theestimated losses of air content. (About 1.5% of increase in air content was related to thechemical shrinkage that takes place during the hardening of the cement paste.) Figure 2 givesthe strength versus w/c of the concretes. Besides an increase with lower w/c, a substantialincrease of strength was observed for silica fume concretes. At early ages the efficiency factorof silica fume is quite large, perhaps as high as 7 at 28 days age, but then decreasing with theage of the concrete. After 7 years no effect at all of silica fume on the compressive strengthwas observed /17/.
3.2 Internal relative humidity, RH, in concrete dependent on the curing temperature
Figures 3-5 show the difference in RH between curing at 20.5 C and 23 C compared with18.5 C (ASTM-calibration /18/). Figure 6 shows that a small average effect of curing at 20.5C was observed. At 23 C RH was on average 0.5% lower than RH with curing at 18.5 C,i.e. the effect of a moderate temperature change on RH was small (hardly detectable). Table 1
4gives the standard deviation and the average difference in RH of the measurements. Themaximum standard deviation was 1.6% (curing at 18.5 C) and the maximum average standarddeviation 0.7% (independent of curing temperature and measured at 20.5 C).
In the fre s h s ta te L o s s e s o f a ir A fte r cur ing
32 L 32 N 32 NS 38 L 38 N 38 NS 50 L 50 N 50 NS
Figure 1. Estimated losses of air content in the concretes in the fresh state and after curing. L=low-alkali cement, N = normal-alkali cement, NS= N + 5% silica fume, 32= w/c (%).
32 L 32 N 32 NS 38 L 38 N 38 NS 50 L 50 N 50 NS
W a te r-ce m e nt ra tio ( % ), ce m e nt ty p e
18 C 20 C 23 C
Figure 2. Compressive cylinder strength versus w/c of the concretes. L= low-alkali cement, N= normal-alkali cement, NS= N + 5% silica fume, 32= w/c (%).
32L 3 2 N 3 2 N S 38L 3 8 N 3 8 N S 50L 5 0 N 5 0 N S
W a te r-ce m e nt ra tio (% )
20 C 23 C
Figure 3. Alteration of RH with curing at 20.5 C and 23 C compared with curing at 18.5 C(measurement performed at 18.5 C).
32L 32N 32NS 38L 38N 38NS 50L 50N 50NS
Water-cement ratio (%)